B2O3 Content on the Sintering Basic Characteristics of Mixed Ore Powder of Vanadium-Titanium Magnetite and Hematite

/e sintering basic characteristics of iron ore play a key role in the process of sintering. In this study, the effects of B2O3 on the assimilation characteristics, softening temperature, fluidity of liquid phase, compressive strength of bonding phase, and microstructure of the mixed fine powder of hematite and vanadium-titanium magnetite (H-VTM) are studied. Results show that B2O3 content from 0%–5% (wt%) could improve the assimilation characteristics of the H-VTM and increase the amount of the liquid phase. /e liquidity of the bonding phase index (LBPI) of the H-VTM increases from 3.7 to 24.2. When B2O3 content exceeds 2%, the diameter of the pore in the H-VTM sintered samples enlarges. However, the compressive strength gradually decreases. Boron and calcium-magnesium-aluminium elements are abundant in the bonding phase, which can reduce the formation of calcium silicate and perovskite in H-VTM sintered samples.


Introduction
With the rapid development of the steel industry, the supply of high-quality iron ore is insufficient, so the vanadiumtitanium magnetite (VTM) with sufficient reserves is highly needed. e extraction of iron, vanadium, titanium, and other elements in VTM has remarkably progressed, and its industrial-scale production is still dominated by the blast furnace ironmaking process. e primary raw materials for the blast furnace are vanadium-titanium sinter and vanadium-titanium pellets [1,2].
Vanadium-titanium sinter is the raw material for the blast furnace, and there are still many difficulties in the production of vanadium-titanium sinter. As increasing the proportion of VTM in sintering, the amount of the liquid phase and the liquid-phase bonding force both decrease. Resulting in a lower yield and drum strength of vanadiumtitanium sinter, the production volume of small size sinter also increases. Low-temperature reduction pulverization index (RDI −3.15 ) of the vanadium-titanium sinter is significantly higher than the sinter without vanadium-titanium magnetite [3,4].
Zhou et al. [5] revealed that enhancing granulation improved the breathability of the sintering layer, and the increase in oxygen potential could multiply the mass fraction of calcium ferrite in the sinter, including mineral composition, yield, and quality [6]. D. G. Jiang et al. [7] proposed a new idea based on the complementary mineralization of the assimilation characteristics and liquid phase fluidity. ey confirmed the feasibility of mineralization based on the sintering basic characteristics of iron ore by optimizing the mineralization method and the sinter pot test. Xu et al. [8] confirmed that the low-temperature reduction pulverization index was improved, and the reduction index was enhanced by 2.6% when the content of iron concentrate rich in boron and magnesium in the vanadium-titanium sintering mixture approached 5%. Chu et al. [9][10][11][12] determined that economic indicators such as vertical sintering speed, yield, drum index, sintering cup utilization coefficient, and low-temperature reduction pulverization index initially increased and subsequently decreased with increasing mass ratio of boron ore. Hao [13] found that the low-temperature reduction pulverization index and drum strength of the sintered ore increased, and the reduction index, softening temperature, and softening remain unchanged after boric acid and calcium chloride were added. Zhao et al. [14,15] observed that adding a certain amount of boron-iron concentrate to the vanadium-titanium sinter could make full use of B 2 O 3 , as a result, the liquid phase of the sinter increased, the consolidation process improved, and the metallurgical properties of the sinter also enhanced.
Ren et al. [16,17] researched the influencing pattern of different B 2 O 3 contents on the mineral phase of high-titanium-type VTM and the qualities of sinter; they pronounced that B 2 O 3 was mainly deposited in the 2CaO•xSiO 2 •2/3 (1 − x) B 2 O 3 phase of vanadium-titanium sinter and B 2 O 3 effectively inhibited the precipitation of CaTiO 3 and 2CaO•xSiO 2 •2/3 (1 − x) B 2 O 3 and promoted the precipitation of iron-containing mineral phase.
In summary, we find that adding boron slime, boric acid, and boron-iron concentrate could improve the strength and the metallurgical performance of sinter and reduce the lowtemperature pulverulent ratio, which is conducive to the blast furnace. It is not difficult to find that boron oxide plays a very important role in the sintering process. However, existing researches mainly focus on the effect of boron oxide on the macroperformance of vanadium-titanium sinter. Studies on the influence of B 2 O 3 on the sintering basic characteristics of mixed ore powders using vanadium-titanium fine powder as the main raw material are rarely reported. Especially the researches on the influence mechanism of B 2 O 3 on the sintering basic characteristics of mixed ore powder of vanadium-titanium magnetite and hematite have not been reported so far.
Hence, in this work, according to the actual production of mineral types and proportions in southwest China. Experimental samples are mixed with VTM concentrate and Australian hematite powder with a specific mass ratio (8 : 2), and this particular mixture powder is called H-VTM. e effects of B 2 O 3 content on the assimilation characteristics, melting temperature, liquidity of liquid phase, compressive strength, and microstructure changes are studied. e influences of different B 2 O 3 contents on the sintering basic characteristics of H-VTM sintering samples are obtained. e mechanism of B 2 O 3 affecting the sintering process of vanadium-titanium magnetite and hematite is also clarified. Meanwhile, it is possible to find a new method for the recycling of B 2 O 3 in boron-containing solid wastes.

Raw Materials.
e chemical composition of the sintered raw material is shown in Table 1. Based on actual production situation, the mixed mineral powder used in this study composes of hematite powder and vanadium-titanium magnetite powder with a mass ratio of 2 : 8. e particle size of hematite powder and vanadium-titanium magnetite powder is both less than 74 μm. All the other reagents used in the experiments are of analytical grade.

Assimilation Characteristics.
e assimilation characteristics experiment is shown in Figure 1. H-VTM and CaO are made into a mixed ore powder sample at 6000 N pressure, with a diameter of 8 mm and CaO sample with a diameter of 15 mm. e mixed ore powder sample was placed on top of the CaO sample and then placed into the sintering device to roast at 200°C in a specific heating system. e heating rate is 10°per minute until the end of the assimilation. Afterwards, the samples were naturally cooled and removed from the device. e assimilation characteristics were characterized at the temperature at which the contact angle between the H-VTM sample and the CaO sample began to change. e assimilation characteristics are used to characterize the difficulty of the reaction between iron ore powder and calcium oxide.

Melting Temperature.
e experiment of melting temperature is shown in Figure 2. e chemical composition of the samples ensured the binary basicity R 2 of 2.0. A mixed sample (1.00 g) is placed in a 3 mm × 3 mm mould to make into the sample. en, it is placed on a corundum gasket. e well-made sample is heated with a particular heating system; the melting of the column is observed to determine its melting temperature.

Compressive Strength of Bonding Phase.
e experiment of the compressive strength of the bonding phase is shown in Figure 3. e chemical composition of the samples ensured the binary basicity R 2 of 2.0. Every mixed sample (3.00 g) is placed in a Φ8 mm × 8 mm mould. e samples are placed in the heating furnace under an air atmosphere and heated at 1250°C for 30 min. After heating, the specimens are moved out from the furnace and air-cooled to ambient temperature. Four sintered samples are selected for the compressive strength test. e average compressive strength is used to characterize the bonding phase strength.

Fluidity of Liquid Phase.
e experiment of the fluidity is shown in Figure 4. e liquidity of the bonding phase index (LBPI) is calculated according to the equation as follows: where S * represents the ratio of the increased area of the sample to the original area of the sample after heating and flowing and S 0 and S 1 are the vertical projection areas before and after flowing. e chemical composition of the samples ensured the binary basicity R 2 of 2.0. A mixed sample of 1.00 g is placed in a Φ8 mm × 8 mm mould and heated at 1350°C for 30 min. After the samples cooled, every sample is removed and     Figure 5, the sample without B 2 O 3 began to assimilate at 1359°C, but the assimilation temperature decreased to 1205°C when the B 2 O 3 was 5.00% (wt%). is result indicated that adding B 2 O 3 could improve the assimilation characteristics of H-VTM. B 2 O 3 has a low melting point (450°C), which could form a low-melting-point chemical compound and promote the formation of the liquid phase. For instance, the reaction of B 2 O 3 with CaO and SiO 2 can form 2CaO·B 2 O 3 ·SiO 2 whose melting point is 901°C. is reaction could effectively inhibit the formation of calcium orthosilicate (2CaO·SiO 2 ). B 3+ is quickly diffused into the crystals of calcium orthosilicate (2CaO·SiO 2 ) and inhibits multiphase transformation of calcium orthosilicate. is reaction is described in the subsequent microstructure analysis.

Sintering Basic Characteristics of H-VTM with Different B 2 O 3 Contents. In
As is shown in Figure 5, when the mass ratio of B 2 O 3 increased from 0.00% to 5.00%, the melting temperature decreased from 1504°C to 1453°C. When increasing the amount of B 2 O 3 , the melting temperature of H-VTM decreased obviously. In the whole process, adding B 2 O 3 was conducive to the improvement of the capacity of the liquid phase inside the sintered samples. e LBPI of the H-VTM increased significantly from 3.70 to 24.2.
is trend was consistent with the results which were calculated using the reaction module and the equilibrium module of FactSage 7.1 software. e calculation conditions were based on R 2 at 2.0 and carbon mass ratio at 3.5% under standard atmospheric pressure and air atmosphere. e chemical composition of the H-VTM was introduced in the reaction and the equilibrium module as input data. e amount of B 2 O 3 was increased from 0.00% to 5.00% with a step size of 1.00%. e temperature was increased from 1000°C to 1600°C in a step of 50°C. e average compressive strength of H-VTM fluctuated significantly with the rise of B 2 O 3 . e compressive strength was 531 N/P without B 2 O 3 . e compressive strength grew significantly with the increase of B 2 O 3 content, peaking at 857 N/P with B 2 O 3 content at 2.00%. As the B 2 O 3 ratio further increases, the compressive strength dropped sharply, reaching its lowest point at 356 N/P with B 2 O 3 ratio at 5.00%.
In Figure 6, at the same mass ratio of B 2 O 3 , the amount of liquid phase in sintering continuously increased with the increase of temperature, especially when the temperature exceeded 1210°C. At the same temperature, the amount of liquid phase of the sample with a high percentage of boron oxide was significantly more than the sample with lower ones. When the ratios of B 2 O 3 were 0.00%, 1.00%, 2.00%, 3.00%, 4.00%, and 5.00%, the ratios of the liquid phase were 15.74%, 25.32%, 32.43%, 39.42%, 44.73%, and 51.36%, respectively. B 2 O 3 could react with CaO, SiO 2 , MgO, and Al 2 O 3 to form mineral phases with a low melting point. Besides, the melting point of B 2 O 3 is low (450°C). erefore, B 2 O 3 initially transformed into the liquid phase. Overheating reduced the liquid viscosity and quickly form a certain amount of liquid phase, which was beneficial for diffusion during sintering. As a result, the amount of liquid phase of H-VTM improved with the increase of the ratio of B 2 O 3 .

Microstructure of H-VTM with Different B 2 O 3 Contents.
e X-ray diffraction (XRD) is used to investigate the phases changes of the sintered samples. As is shown in Figure 7, after heating samples at 1250°C for 30 min, by contrast, the diffraction peaks of Fe 3 O 4 and CaO·Fe 2 O 3 increased as the B 2 O 3 mass ratio increased. e addition of B 2 O 3 could inhibit the formation of 2CaO·SiO 2 and promote the formation of CaO·Fe 2 O 3 . is scene is shown in Figure 8. Before 1100 o C, the 2CaO·SiO 2 content grew continuously with the increase of the B 2 O 3 mass ratio. It reached its highest value when the addition amount of B 2 O 3 is 5.00% at 1100°C. e microstructures of the samples with different content of B 2 O 3 were observed using a scanning electron microscope (SEM) equipped with an energy-dispersive X-ray spectroscope (EDS). In Figure 9, as the amount of B 2 O 3 increased, the bonding phase (the bright white part) in the  e scanning results of the sintered sample with 5.00% B 2 O 3 are shown in Figure 10. Hematite was mainly distributed in a fish-bone shape. Silicon, calcium, and aluminium were combined and distributed in the bright white area and formed a bonding phase. Titanium and iron were concentrated, producing the main iron base phase.
SEM-EDS was carried out on the cooled sample with 5.00% B 2 O 3 , as is shown in Figure 11. e EDS analysis results from point A to C with 5.00% B 2 O 3 are shown in Table 2

Conclusions
e assimilation characteristics, melting temperature, fluidity of the liquid phase, compressive strength of the bonding phase, and microstructure of H-VTM with different B 2 O 3 were studied through different methods: B 2 O 3 reduces the assimilation temperature of H-VTM and enhances its assimilation characteristics. As the amount of B 2 O 3 increases, the melting temperature of H-VTM decreases, as well as LBPI. e addition of B 2 O 3 can increase the amount of liquid phase and enhance the fluidity of the liquid phase. B 2 O 3 (<2.00%) improves the bonding phase strength of sintering samples, but the diameter of the pore in H-VTM enlarges when the amount of B 2 O 3 is over 2.00% and the number of the pore increase. us, the H-VTM microstructure becomes more porous, and its compressive strength decreases. Boron and calcium-magnesium-aluminium concentrated in the bonding phase can reduce the formation of calcium silicate and perovskite in the mixed samples of vanadium-titanium and hematite.

Data Availability
e data used to support the findings of this study are available from the corresponding author upon request.

Conflicts of Interest
e authors declare no conflicts of interest.   Journal of Chemistry